Cellular Ceramics by Direct Foaming of Emulsified Ceramic Powder Suspensions
Post on 20-Jul-2016
Cellular Ceramics by Direct Foaming of Emulsified Ceramic PowderSuspensions
Suelen Barg,w Christian Soltmann, Miria Andrade, Dietmar Koch, and Georg Grathwohl
Ceramic Materials and Components, University of Bremen, D-28359 Bremen, Germany
A new direct foaming method to produce macroporous cellularceramics using surfactants as foam stabilizers is presented. Thetechnology relies on the transition of a stabilized aqueous ceramicpowder suspension containing a homogeneously dispersed alkaneor airalkane phase into cellular ceramics. The stabilization ofthe powder suspension and the emulsion is realized with partic-ular emphasis on the interaction of both mechanisms providingenduring stability of the system up to high foaming degrees. An-ionic, cationic, and nonionic surfactants were studied with theirstabilization and foaming effects. The presence and inuence ofair bubbles was proved to be of negligible importance. Foaming isthen provided by the evaporation of the emulsied alkane drop-lets, leading to the expansion of the emerging foam and givingrise to solids foams with cell sizes from 0.5 to 3 mm and poros-ities up to 97.5% after sintering. The microstructures of theseligree ceramics are stable and rigid with dense struts anduniform distributions of the solid phase and the porosity.
HIGH-performance ceramics with cellular microstructuresnd their applications in many different elds of moderntechnologies. Owing to their specic properties such as highpermeability, high surface area, high-temperature stability, lowweight, and low thermal conductivity, the development of highlyporous ceramics has attracted increasing interest in recent years.These applications include ltration of molten metals and hotgases, thermal and acoustic insulation, light-weight structuralcomponents, catalytic carriers, support for fuel cells, electrodes,sensors, bioreactors, radiant burners as well as scaffolds forbone replacement.16
The functions of these advanced materials and componentsare based on the presence of controlled porosity. This is relatedto the main porosity parameters as total porosity, pore size dis-tribution, pore morphology, connectivity between the pores,specic surface area, and their effect on mechanical properties.The tailored microstructures required by the specic applica-tions have to be realized by adjusting the synthesis parametersand the processing routes.The processing method has a decisive inuence on the micro-
structure and the properties of the material. Different manufac-ture processes have been used to produce porous ceramics withcontrolled properties. The main processes presently availablecan be classied into replica, sacricial template, and directfoaming techniques. The essential features of these methodshave been reviewed recently by Studart et al.2
The most common process for producing ceramic foams isthe replica technique, which consists in the impregnation of apolymeric sponge (typically of polyurethane) with a ceramicslurry or a precursor solution, followed by the removal of excess
slurry, pyrolysis of the polymeric substrate, and nally sinteringin an appropriate atmosphere and temperature for solidicationof the foam.7,8 Therefore, the ceramic foam replicates the orig-inal organic polymer structure. This technique allows to produceporous ceramics with cellular porosity and pore sizes rangingfrom approximately 200 to 3 mm.9 The difculty of slurry im-pregnation limits the realization of smaller cell sizes. The strutscontain central holes, which result from the burning out of thepolyurethane template as well as microcracks and pores. Fur-thermore, the replication technique generates a large amount ofCO2 during ring due to decomposition of organic com-pounds.79 Suitable biogenic porous structures have also beenused as templates for the realization of cellular ceramics withparticular microstructures that could not be produced by othermethods. Different techniques have been developed for the rep-lication of wood structures in various ceramic materials.10,11
In case of the sacricial template technique, a fugitive phasethat can be removed by a burning,12 decomposition,13 or evap-oration14 process is uniformly dispersed in a ceramic precursor.The desired porosity is then obtained as a residue of the sacri-cial phase. With this technique, one can achieve pore sizes from1 to 700 mm and porosities from 20% to 90%. The microstruc-tures obtained by this technique reect directly the pattern of thesacricial phase.In direct foaming techniques, a ceramic suspension is foamed
by gas incorporation (physical or chemical blowing); the wetfoam is stabilized, dried, and sintered. Extremely high porositiesup to 97% can be obtained. The expenditure for this method islow and its exibility is high in terms of chemical compositionand adjustment of the nal microstructure. The key aspects arethe stabilization and consolidation mechanisms. Wet foams arethermodynamically unstable systems in which processes likedrainage of the liquid phase and gas bubble coarsening lead tofoam degradation and nal destruction. Drainage correspondsto the ow of the liquid phase due to the gravity effect. Reducingthe amount of the liquid phase results in a closer approach of thebubbles, which leads to their coalescence. Diffusion of gas oc-curs between bubbles of different sizes and consequently differ-ent concentrations of gas due to the difference in Laplacepressure between them (Ostwald ripening).2,1517 These mecha-nisms of foam degradation are driven by the reduction of theGibbs free energy of the system. It is then of fundamental im-portance to activate further stabilization effects in order to con-trol the natural evolution of the foamed powder suspensions andto provide adjustment of the cellular ceramic microstructure.Surfactants can be used as surface-active agents for the stabi-
lization of wet foams. These long-chain amphiphilic moleculesadsorb at the gas bubble surfaces with their hydrophilic tail incontact with the aqueous phase. The foaming ability of a sur-factant is related to its effectiveness to lower the interfacial energyor the surface tension at the gasliquid interface. Their chemistry,in terms of molecular weight, polarity, and critical micelle con-centration, can signicantly inuence the emerging microstruc-ture of the foamed suspension. Surfactants are classiedaccording to the hydrophilic group as anionic, cationic, nonion-ic, and amphoteric.15 Ceramic foams stabilized by surfactants arereported to have pore sizes from 35 mm up to the mm scale.1822
J. Hallorancontributing editor
wAuthor to whom correspondence should be addressed. e-mail: email@example.comManuscript No. 24298. Received February 8, 2008; approved May 19, 2008.
J. Am. Ceram. Soc., 91  28232829 (2008)
r 2008 The American Ceramic Society
Colloidal particles can also be used as foam stabilizers toproduce ultrastable wet foams.17,2328 Recently, Gonzenbachet al.2326 have developed a method that manages the surfacemodication of highly concentrated colloidal particles in sucha way that a high concentration of small air bubbles can bepreserved against destabilization. With this method, smallerpore sizes (10300 mm) can be achieved in the cellular ceramicmicrostructures. Besides the reduction of pore sizes, the particlestabilization method allows straightforward consolidation anddrying processes leading also to remarkable compressivestrength of the resulting porous ceramics.A direct foaming process is described in this paper, with an
emulsied ceramic powder suspension being conditioned for thispurpose by emulsifying a homogeneously dispersed alkane orairalkane phase in the stabilized aqueous powder suspension. Incontrast to the more conventional direct foaming methods wherefoaming is achieved during stirring by incorporation of air bub-bles into the suspension, foaming is provided here by evapora-tion of the emulsied alkane droplets. This process leads to atime-dependent expansion of the emerging foam in a mold, withthe shaping of the cellular part being accomplished in situ duringthe process. This autonomous foaming process then allows highexibility in the production of ceramic parts with very highporosities including gradient structures and complex shaping.Foaming proceeds while the conditions for stabilization are
fullled for both parts of the system, namely the powdersuspension and the alkane emulsion. The rising foam then hasto be consolidated before destabilization processes can lead tofoam degradation. Because this consolidation process is mainlyprovided by drying the kinetics of foaming, bubble expansion,foam aging, and drying have to be considered as concurrentprocesses with their individual dependencies on the parametersof the system and the process. A general description of the directfoaming process has been presented in a previous work.18,19 It isthen the objective of this paper to identify the parameterscontrolling the transition from an emulsied suspension to aceramic foam, in particular, the effects of different surfactantsand stabilization factors on the foaming process, the inuence ofair introduction, and combined effects on the microstructure ofthe ceramic foams emerging from this process. While themethod is described here for alumina foams, this techniquemay also be applied to other oxide and nonoxide ceramicsand even metals depending on the adjustment of dispersionagents and surfactants for the different powder surface chemis-tries. As surfactants provide highly efcient means to stabilizegasliquid or liquidliquid interfaces, their actual charging stateis of particular interest for this foaming process, taking intoaccount that cationic and anionic surfactants are expected to actas better foaming agents compared with nonionic surfactants.29
Commercially available surfactants are then used for the prep-aration of emulsied suspensions and tested in terms of foamingability and foam growth as well as their inuence the nalmicrostructure of the ceramic foams.
II. Materials and Methods
Powder suspensions were prepared using deionized water and a-Al2O3 powder (Alcoa CT 3000 SG, Alcoa, Frankfurt, Germany)with an average particle diameter (d50) of 500 nm and a specicsurface area of 7.5 m2/g. A low-molecular-weight (320 g/mol)polyacrylic acid commercially available as Dolapix CE-64
(Zschimmer & Schwarz, Lahnstein, Germany) was added as anegatively charged electrosteric dispersion agent to stabilize thesuspensions. The effect of anionic, nonionic, and cationic long-chain surfactants (Table I) on the stabilization of the alkaneand airalkane bubbles in the emulsions was investigated. Theaddition of these surfactants had to take into account the z po-tential and isoelectric point (IEP) of the alumina suspension.Cationic surfactants could only be applied under acidic condi-tions (pH 5.5) where the z potential is high, while anionic andnonionic surfactants were used under alkaline conditions (pH9.5) where the strong negative z potential was provided by thedispersion agent. pH 5.5 was adjusted by hydrochloric acid 1 N(Riedel-de Haen, Seelze, Germany).
(2) Preparation of the Alkane Emulsion in the PowderSuspension
For the production of the cellular ceramics, the rst step is thepreparation of a stabilized alumina powder suspension. Thisstep is followed by the formation of an emulsion as a homoge-neous dispersion of an alkane phase or an alkane phase in com-bination with air bubbles in the alumina suspension. For thispurpose, surfactants as stabilizers and the alkane phase areadded after the stabilized alumina suspension is prepared. Incase of anionic and nonionic surfactants, the stabilized powdersuspensions were prepared as follows: 42 vol% of alumina pow-der was slowly added to deionized water containing DolapixCE-64 (0.74 wt% related to alumina) as a dispersion agent un-der vigorous mixing. Dispersion and homogenization was car-ried out in a laboratory mixer (Dispermat LC, VMA GetzmannGmbH, Reichshof, Germany) with a 30 mm dispersing tool op-erating at a mixing velocity of 2500 rpm for 20 min. In formerexperiments,18,19 the optimal powder dispersion was investi-gated and attributed to the efciency of this electrosteric disper-sion agent.For the production of foams stabilized with cationic surfact-
ants, the suspensions were prepared at pH 5.5 with HCl wherethez potential is found to be sufciently high for stabilization ofthe alumina suspension. The other parameters are the same asthose described for anionic and nonionic surfactants. After-wards, the suspensions were subjected to deaeration to removeundesired entrapped bubbles. This procedure was performed ina container under reduced pressure (5 kPa).Subsequently, 5.5 vol% heptane was added to the ceramic
suspension, together with 0.83 vol% of different surfactants(Table I), thereby dening Vi as the initial volume of the com-bined system. Mixing is then achieved by mechanical stirring for2.5 min at 2500 rpm. This preparation step of the alkaneemulsion in the powder suspension is accompanied by airincorporation into the system if the mixing procedure occursin ambient air. This happens because the surfactants decreasethe gasliquid surface tension and a rst volume increase isachieved by this process step. This volume increase of the emul-sied suspensions during mechanical stirring was determined bythe foaming ability coefcient Fa5Vf/Vi, with Vf describing thevolume of the emulsion after air incorporation by mechanicalstirring for 2.5 min.The suspensions containing the different surfactants were
emulsied in ambient air but also under reduced pressure atroom temperature to avoid the abundant incorporation of airbubbles. A moderately reduced pressure of 10 kPa was chosenwith respect to the evaporation of heptane, which has a vaporpressure of 4.6 kPa at 201C.
Table I. Properties of the Surfactants Used as Foaming Agents
Type Commercial notation Producer Molecular weight (g/mol) Molecular formula
Anionic Lutensit AS 2230 BTC 671.3 C12O(CH2CH2O)2 5SO3NaCationic B8879 Sigma 448.1 C27H42ClNO2Nonionic Lutensol ON80 BASF 358 C18H37(OCH2CH2)2OH
2824 Journal of the American Ceramic SocietyBarg et al. Vol. 91, No. 9
(3) Foam Formation, Setting, and Sintering
The emulsied suspensions were poured in quantities of 12 and26 g into plastic round molds with diameters of 50 and 80 mm,respectively, and a height of 15 mm. The following autonomousfoaming process was realized in a clima chamber (TerraUniversal, Fullerton, CA) under controlled temperature andhumidity (231C and 65%). Foaming proceeds as a consequenceof the evaporation of the alkane phase resulting in the growth ofthe stabilized alkane bubbles and in a volume increase of thefoam (Fig. 1). The resulting foamed green body possesses a tightcylindrical form with a cross section corresponding to the mold.The foaming growth was evaluated under controlled tempera-ture and humidity conditions dependent on the surfactant usedand the presence of air bubbles during 4 h. The growth of thefoam with time was calculated by (htho)/ho where ho is the ini-tial height of the freshly poured samples and ht is the height ofthe foams after a given time. After the consolidation, the al-umina foams were dried and sintered at 15501C for 2 h.
(4) Characterization Methods for Suspensions, EmulsiedSuspensions, and the Sintered Foams
Zeta potential experiments (DT-2000, Dispersion technologyInc., Bedford Hills, NY) were undertaken with alumina suspen-sions (5 vol%), with and without Dolapix CE-64 (0.74%) as adispersion agent, in order to determine the stabilization state ofthe suspensions.Immediately after mechanical stirring, samples of the emul-
sied suspensions were transferred into closed Quartz cells (Hell-ma, Mullheim/Baden, Germany) or opened recipients (when theinvestigation of the bubble growth was intended) and subse-quently analyzed by uorescence microscopy. The alkane phasewas dyed with Pyrene (Fluka, Steinheim, Germany), making the
alkane droplets uorescent at an emission wave length lEm of375 nm. With this technique, it was possible to distinguish thealkane droplets and airalkane bubbles from the alumina sus-pension. Droplet and bubble size distributions were measured inclosed emulsied suspensions composed of 0.83 vol% anionicsurfactant and 5.5 vol% heptane produced under reduced pres-sure and in ambient air. For each condition, 100 droplets orbubbles were individually measured for statistical analysis withthe use of Axio Vision LE image analysis program.The cellular network and the microstructure of the sintered
ceramic foams were analyzed by scanning electron microscopy(Camscan 24, Cambridge, England) as well as by computer X-ray tomography (mCT 40 Scanco medical, Bassersdorf, Switzer-land). Therefore, ceramic foams were cut and cell size distribu-tions were directly obtained from planar sections. As the foamswere rigid enough and no embedding was necessary, the win-dows were easily distinguished from the cell architecture. Cellsize, window opening, and strut thickness were individuallymeasured with the help of an image analysis program (Analy-SIS). For each condition, two regions per sample in two sampleswere chosen and digital images were taken for statistical anal-ysis. The volumetric density rv of the foams was determinedfrom the mass and dimensions of the sintered bodies. The po-rosity P was then calculated as P5 1rv/rt, with rt (3.9 g/cm3)corresponding to the theoretical density of alumina.
III. Results and Discussion
(1) Stabilization of the System
For successful foaming of the system, the suspensions and theemulsions had to be sufciently homogenized and stabilized asdescribed in Section II(2). The effects of the suspension stabili-zation agent and the foaming agents are taken into account in away to control their interaction and consequently to prevent thedestabilization and coagulation of the system. Therefore, in caseof anionic and nonionic surfactants, the alumina suspension wasnegatively stabilized while the alumina particles were positivelycharged when the emulsion was stabilized by cationic surfactants.The z potential curve of the alumina suspension in Fig. 2 showsthat at pH 5.5 (by which the suspension is prepared), the particlesurfaces are positively charged which enables the use of the cat-ionic surfactant. On the hand side, the adsorption of (COO)anions on the alumina surface shifts its IEP to 4.65, resulting in anegative surface charge of the alumina particles at pH 9.5, bywhich these suspensions are prepared. In this case, the suspensionstabilization is adequate for the use of anionic and nonionicfoaming agents. In all cases, the suspensions and emulsions wereefciently prepared without coagulation in the systems.
Fig. 1. Autonomous foaming process: (a) emulsied alumina powdersuspension freshly poured into the mold; (b) wet foam formed after 3 hat 231C and 45% humidity.
2 4 6 8 10 12 1450
40 0% Dolapix 0.74% Dolapix
Fig. 2. Zeta potential of alumina suspensions as a function of pH with-out and with a negatively charged dispersion agent Dolapix CE-64. Thesuspensions were prepared with 5 vol% of alumina.
September 2008 Cellular Ceramics by Direct Foaming 2825
The emulsied suspensions closed in quartz cells were analyzedimmediately after mechanical stirring under uorescence micros-copy. The size distributions of the alkane droplets and theairalkane bubbles in the emulsied suspensions are presentedin Fig. 3. The alkane droplet size distribution produced underreduced pressure in the emulsied ceramic suspension rangesfrom 2.5 to 6 mm, with a mean droplet size (d50) of 4.13 mm.When ambient air is present during the emulsication process, thealkane distribution is modied and, besides the small alkanedroplets, larger alkaneair bubbles are observed up to 40 mm.This broadening is caused by stirring under ambient air, leadingto a rst foaming step as described later (Fig. 6).
(3) The Foaming Process
The transition of the emulsied ceramic suspension to the wetfoam starts as soon as the emulsication process is completed.The bubble size evolution of an emulsied suspension contain-ing 5.5 vol% heptane and 0.83 vol% anionic surfactant emul-sied in ambient air is shown in Fig. 4 using uorescencemicroscopy. Foaming is investigated here in a model experi-ment leading to images that illustrate the foaming progress ofthe emulsied suspension in an opened recipient. The systemcontains small heptane droplets and larger airheptane bubblesat the start of foaming as indicated in Fig. 4(a). The transfor-mation of the alkane phase from liquid to gas directly after themixing process is accompanied by the expansion of bubbles dueto its high vapor pressure (Fig. 4(b)). Simultaneous with bubbleexpansion, other physical processes assist the bubble growth,decreasing thereby the free energy of the system. Some smallheptane bubbles disappear due to gas diffusion from smallerto larger bubbles as a result of the Laplace pressure gradientbetween them (Ostwald ripening). The number of bubbles isreduced while their size increases. Other bubbles coalesce andgrow by thinning and breaking of the lm surrounding them.These effects can be observed from the recorded images resultingin a rapid bubble size increase. After 3 min (Fig. 4(c)) under themicroscope, the plateau borders are well dened and the foam-ing process in this model sample approaches its completion.The setting of the foam is assisted by advancing drainage
processes at plateau borders and thin lms, evaporation of theliquid phase (drying), and consequent rupture of the bubblemembranes. Consequently, the concurrence between the bubbleexpansion kinetics and the setting of the structure controlsthe foam cell size. Moreover, parameters like surfactant nature,
vapor pressure and content of the vaporizing components,temperature, and humidity also inuence these mechanisms.18,19
The foaming process proceeds continuously from the top tothe bottom of the poured suspension. While alkane droplets inthe top region evaporate and grow, new droplets are simulta-neously starting the foaming process in the lower parts until thewhole volume of the emulsion is converted into a stable foam.Three stages of the foaming process can be recognized as illus-trated in Fig. 5. The emulsied suspension is represented bystage (a). The alkane droplets located at the upper parts of theemulsion start evaporating, giving rise to spherical bubblespresent at stage (b). The formation of polyedric structures char-acterized by thin lms at the interfaces of touching cells and theso-called plateau borders at the intersection of three interfaciallms is rst reached in the top layer and denes stage (c). Thisstage represents the transition of the growing to the stable foamand corresponds to the situation presented in Fig. 4(c).
(4) Inuence of Surfactants on the Foaming Process and theMicrostructure
The foaming ability coefcient Fa of the three different surfact-ants used is shown in Fig. 6. The cationic surfactant shows ahigher ability of air stabilization in the system, followed byanionic and nonionic surfactants. Primarily, the ability of afoaming agent to incorporate large quantities of air into theemulsied suspension depends on the surfactants effectivenessin reducing the surface tension of the system.
Emulsification in ambient air under reduced pressure (10 kPa)0
0 5 10 15 20 25 30 35 40 45
Fig. 3. Effect of partial pressure during mixing (2.5 min) on the alkanedroplet and airalkane bubble size distribution in emulsied aluminasuspensions containing 5.5 vol% heptane and 0.83 vol% anionic sur-factant. Size measurement was enable by uorescence microscopy underclosed recipient conditions.
Fig. 4. Bubble growth in alumina powder suspension emulsied (5.5vol% heptane and 0.83 vol% anionic surfactant) in ambient air as il-lustrated via uorescence microscopy. (a) Samples freshly poured in anopened recipient; (b) after 1 min and (c) after 3 min. The inset in (a)shows the small alkane droplets. The larger dispersoids correspond toairalkane bubbles. In (c), the plateau borders can be seen.
2826 Journal of the American Ceramic SocietyBarg et al. Vol. 91, No. 9
After pouring the emulsied suspension into the mold, thefoaming process starts immediately as being driven by the au-tonomous evaporation of the alkane phase. As shown in Fig. 7,the foaming rate is higher in case of the anionic surfactant, fol-lowed by the cationic and nonionic surfactants if the emulsion isprepared under reduced pressure (Fig. 7(a)) or in ambient air(Fig. 7(b)), leading to the incorporation of air bubbles.The foams emulsied under reduced pressure grow at lower
foaming rates at the beginning that increase with time(Fig. 7(a)). For the foams emulsied in ambient air, the oppo-site effect takes place, with higher foaming rates at the initialstage being reduced during the process (Fig. 7(b)). Air bubblespresent at the start of foaming may be effective in acceleratingthe autonomous foaming process in its early stage becausepreexistence of gasliquid interfaces is provided in this case.The lowest foaming rates are observed in the systems with
nonionic surfactants, the foam growth being dened as Dh/ho,with the initial height ho of the suspension level in the mold(Fig. 7). After a rather low foam growth of about 150%,the foaming process fades away in nonionically stabilizedsuspensions emulsied in ambient air, while the other samples,
in particular, the anionically stabilized systems, revealed the factthat the foaming process is not completed after 4 h; in contrast,foam growth, albeit with differing foaming rates, is still con-tinuing and leads in the system with the highest foamability(anionic surfactant, emulsication under reduced pressure) to a
Emulsification under reduced pressure
Anionic Cationic Nonionic
0 50 100 150 200 250Time (min)
0 50 100 150 200 2500
600 Emulsification in ambient air
Anionic Cationic Nonionic
Fig. 7. Autonomous foaming of emulsied alumina suspensions pre-pared with anionic, cationic, and nonionic surfactants and 5.5 vol% hep-tane in air ambient (a) and under reduced pressure, 10 kPa (b). ho is theinitial height of the emulsied suspension after being poured into the mold.
Fig. 5. The three stages of the foaming process of an emulsied ceramicpowder suspension: (a) alkane emulsion in the powder suspension;(b) transition of emulsion to wet foam; and (c) formation of a polyhe-dral structure (transition to stable foam).
Fig. 6. Foaming ability of emulsied alumina suspensions containing5.5 vol% heptane and 0.83 vol% nonionic, anionic, or cationic surfact-ants mechanically stirred in ambient air for 2.5 min at 2500 rpm.
Fig. 8. mCT analysis of cellular alumina produced from powder suspen-sion emulsied (5.5 vol% heptane and 0.83 vol% nonionic surfactant)under reduced pressure (10 kPa). (Edda SternUniversity of Erlangen).
September 2008 Cellular Ceramics by Direct Foaming 2827
very high foam growth beyond 550% after 4 h of foaming. Thecurves in Fig. 7 could not be extended to a longer durationbeyond 4 h although a further linear progress of the foamgrowth is suggested by the slope of the curves. The reason forthis can be seen in the macroscopic instability and the upcomingnonuniformity of the shape of the foamed body; reliable deter-mination of further foam growth is then not possible anymore.It also has to be noticed that the samples with the highest foamgrowth represent a very high porosity in the range of 90%,approaching the physical limit of the foamability of suchpowder suspensions. If it is possible to transform these wetfoams to ceramic cellular structures by sintering, extremely highporosities beyond 95% are reached under the assumption ofzero shrinkage.The foaming results of Fig. 7 reveal the fact that the anion-
ically stabilized emulsion represents the optimal condition foreffective foaming processes of the alumina suspensions. This re-sult then also yields the suitable state and interaction of thepowder suspension stabilized by the negatively charged disper-sion agent with the anionically stabilized emulsion, therebyfavoring the enduring stability of the whole system during the
most effective foaming procedure. The actual task to providestructural stability during foaming has to be guaranteed by thecell walls of the emerging foam. Their function in providingundamaged thin barriers between the growing gas bubblesdepends on both their strength and resistance against viscousow. It is obvious that these membranes fulll their tasks in amost impressive way when the powder suspension is foamed tosuch high porosity levels.The microstructure of the sintered foams (15501C, 2 h) is
characterized by high porosities between 93 and 97.5 vol% uni-formly distributed throughout the sample with numerous inter-connections between the individual cells. Figure 8 gives animpression of a cellular ceramic part produced with a nonion-ic surfactant under reduced pressure as a mCT-picture. Micro-structural details of the foams produced by anionic, cationic,and nonionic surfactants under reduced pressure are presentedin Fig. 9 including the fracture surface of a single strut underhigher magnication. The homogeneously sintered microstruc-ture of the strut without any pores or voids is illustrated. Thehigh degree of foaming in the anionically stabilized system(Fig. 9(a)) turns out as higher porosities and larger cell sizescompared with the other systems (Figs. 9(b) and (c)). This is alsoquantitatively described in Fig. 10 where cell sizes from 0.5to 3.5 mm are shown with their distributions for the systemsinvestigated. It is also noticeable that more spherical cells andsmaller cell windows are caused by the nonionic surfactant,while the structure of the anionically stabilized sampleapproaches the nal cellular state of polygonization.The foamability and nal cell size of the sintered foam are
mainly attributed to the processes of bubble expansion andcoalescence taking place in the wet foams. These processes occurat signicantly faster rates in the anionic surfactant-basedfoams. Rapid bubble expansion to high foaming degrees is ac-companied by the reduction of the liquid lm thickness, leadingnally to thinner struts, and larger cell and window sizes.While the nal morphology and mean cell size of the foams
produced in ambient air do not show relevant difference fromthe foams produced under reduced pressure, a slightly largerdispersion in the cell size distribution is observed under ambientair conditions. Therefore, the incorporation of air into thesystem changes the foaming rate and slightly decreases thehomogeneity in the cell size distribution, which was alreadydemonstrated by the droplet size distribution (Fig. 3). In otherwords, the foaming process is effective with or without theincorporation of air; this parameter has only limited inuenceon the foaming degree and the nal homogeneity of the foams.
Fig. 9. Macrostructures of cellular alumina produced from powdersuspensions containing 5.5 vol% heptane with addition of anionic (a),cationic (b), and nonionic (c) surfactants emulsied under reduced pres-sure (10 kPa). The foams were formed at 231C and 65% humidity andsintered at 15501C for 2 h. The inset in (a) shows the fracture surface of asingle dense strut.
0.5 1.0 1.5 2.0 2.5 3.0 3.5
Anionic Cationic Nonionic
Cell size (mm)Fig. 10. Cell size distributions of cellular alumina produced from pow-der suspensions containing 5.5 vol% heptane with addition of anionic,cationic, or nonionic surfactants emulsied under reduced pressure (10kPa). The foams were formed at 231C and 65% humidity and sintered at15501C for 2 h.
2828 Journal of the American Ceramic SocietyBarg et al. Vol. 91, No. 9
The foams produced in this work present a rather uniformpore size distribution in the vertical as well as in the horizontaldirection. However, as foaming is a time-dependent process,gradients in porosity and pore size distribution can be realizedby adjusting the foaming conditions and the shape and dimen-sions of the foamed body.
Emulsions containing a homogeneously dispersed alkane or anairalkane phase in a stabilized aqueous ceramic powder sus-pension were efciently prepared and stabilized. With the pro-cessing route based on the transition of the emulsied suspensionto cellular ceramics, it is possible to realize interconnected struc-tures with cell sizes from 0.5 to 3 mm and porosities up to 97.5%.Foaming rate and ability are controlled by the type of long-
chain surfactants used as a foaming agent. The autonomousfoaming process proceeds at faster rates in the anionic surfact-ant-based system, resulting in foams containing thinner struts,and larger cell and window sizes. The effective stabilizationmechanisms of both the powder suspension and the alkaneemulsion provide in their mutual interaction a suitable basefavoring enduring stability of the system up to extremely highfoaming degrees.The incorporation of air into the system increases the foam-
ing rate in the early stage; some broadening of the droplet andcell size distribution is then observed without strongly affectingthe overall foaming degree compared with foaming underreduced pressure.The process described here can also be extended to other
oxide and nonoxide ceramic as well as metallic powders.Corresponding with the large variation of structural parametersobtainable by this method, numerous applications of the cellularceramics as lters for the metal casting industry, catalytic sup-ports, pore burners, matrix for immobilized microorganisms,and scaffolds for tissue engineering are envisaged.
The authors are grateful to DFG for enabling this work within the frame of theGraduate school PoreNet. The contribution of Dr. S. Blindow to the uorescencemicroscopy experiments realized at the Bioceramics group, University of Bremen,as well as the m-CT analysis by Dr. E. Stern, University of Erlangen, are alsogratefully acknowledged.
References1M. Schefer, and P. Colombo (Eds.), Cellular Ceramics: Structure, Manufac-
turing, Properties and Application. Wiley-VCH, Weinheim, 2005, p. 645.2A. R. Studart, U. T. Gonzenbach, E. Tervoort, and L. J. Gauckler, Processing
Routes to Macroporous CeramicsA Review, J. Am. Ceram. Soc., 89 177189 (2006).
3A. Reitzmann, F. C. Patcas, and B. Kraushaar-Czarnetzki, KeramischeSchwammeAnwendungspotenzial monolitischer Netzstrukturen als katalytischePackungen, Chem. Ing. Technol., 78, 88598 (2006).
4L. J. Gauckler, M.M.Waeber, C. Conti, andM. Jacobduliere, Ceramic Foamfor Molten-Metal Filtration, J. Metals, 37  4750 (1985).
5Q. Z. Chen, K. Rezwan, D. Armitage, S. N. Nazhat, and A. R. Boccaccini,The Surface Functionalization of 45S5 Bioglass
-Based GlassCeramic Scaffoldsand its Impact on Bioactivity, J. Mater. Sci.: Mater. Med., 17  97987(2006).
6Q. Z. Chen, I. D. Thompson, and A. R. Boccaccini, 45S5 Bioglasss-DerivedGlassCeramic Scaffolds for Bone Tissue Engineering, Biomaterials, 27, 241425(2006).
7P. Colombo and J. R. Hellmann, Ceramic Foams from PreceramicPolymers, Mater. Res. Innovat., 6, 260 (2002).
8J. Saggio-Woyansky, C. E. Scott, and W. P. Minnear, Processing of PorousCeramics, Am. Ceram. Soc. Bull., 71  167482 (1992).
9S. N. Jayasinghe and M. J. Edirisinghe, A Novel Method of Forming OpenCell Ceramic Foam, J. Porous Mater., 9, 265 (2002).
10C. R. Rambo and H. Sieber, Novel Synthetic Route to Biomorphic Al2O3Ceramics, Adv. Mater., 18  108891 (2005).
11J. Cao, C. R. Rambo, and H. Sieber, Manufacturing of Microcellular,Biomorphous Oxide Ceramics from Native Pine Wood, Ceram. Int., 30,196770 (2004).
12P. Colombo, E. Bernardo, and L. Biasetto, Novel Microcellular Ceramicsfrom a Silicone Resin, J. Am. Ceram. Soc., 87  1524 (2004).
13H. Schmidt, D. Koch, G. Grathwohl, and P. Colombo, MicroMacroPorous Ceramics from Preceramic Precursors, J. Am. Ceram. Soc., 84, 22525(2001).
14D. Koch, L. Andresen, T. Schmedders, and G. Grathwohl, Evolutionof Porosity by Freeze Casting and Sintering of SolGel Derived Ceramics,J. SolGel Sci. Technol., 26, 14952 (2003).
15L. L. Schramm, Emulsions, Foams, and Suspensions: Fundamentals andApplications. Wiley-VCH, Weinheim, 2006.
16J. K. Park, J. S. Lee, and S. I. Lee, Preparation of Porous Cordierite UsingGelcasting Method and its Feasibility as a Filter, J. Porous Mater., 9, 203(2002).
17B. S. Murray and R. Ettelaie, Foam Stability: Proteins and Nanoparticles,Curr. Opin. Colloid Interf. Sci., 9, 314 (2004).
18O. Lavrentyeva and G. Grathwohl, Zellularkeramik aus autarkenSchaumungsprozessen keramischer Suspensionen, Teil 1, Keram. Zeitschr., 2,8893 (2007).
19O. Lavrentyeva and G. Grathwohl, Zellularkeramik aus autarkenSchaumungsprozessen keramischer Suspensionen, Teil 2, Keram. Zeitschr., 4,2605 (2007).
20O. Lavrentyeva, M. Jeske, C. Soltmann, D. Koch, and G. Grathwohl,Verfahren zur Herstellung von anorganischen Schaumen, danach hergestellterSchaum und Verwendung desselben; Patent Registration 102 005 039 774.3,23.8.2005.
21M. Fuji, T. Kato, F. Zhang, and M. Takahashi, Effects of Surfactants onthe Microstructure and Some Intrinsic Properties of Porous Building CeramicsFabricated by Gelcasting, Ceram. Int., 32, 797 (2006).
22S. N. Tan, D. Fornasiero, R. Sedev, and J. Ralston, The Role of SurfactantStructure on Foam Behaviour, Colloids Surf. A: Physicochem. Eng. Aspects, 263,233 (2005).
23U. T. Gonzenbach, A. R. Studart, E. Tervoort, and L. J. Gauckler, Mac-roporous Ceramics from Particle-Stabilized Wet Foams, J. Am. Ceram. Soc., 90 1622 (2007).
24U. T. Gonzenbach, A. R. Studart, E. Tervoort, and L. J. Gauckler, Tailoringthe Microstructure of Particle-Stabilized Wet Foams, Langmuir, 23  102532(2007).
25U. T. Gonzenbach, A. R. Studart, E. Tervoort, and L. J. Gauckler,Ultrastable Particle-Stabilized Foams, Angew. Chem. Int., 45  252630(2006).
26U. T. Gonzenbach, A. R. Studart, D. Steinlin, E. Tervoortand, and L. J.Gauckler, Processing of Particle-Stabilized Wet Foams into Porous Ceramics,J. Am. Ceram. Soc., 90  340714 (2007).
27B. P. Binks, Particles as Surfactants Similarities andDifferences,Curr. Opin.Colloid Interf. Sci., 7, 21 (2002).
28S. Arditty, C. P. Whitby, B. P. Binks, V. Schmitt, and F. Leal-Calderon,Some General Features of Limited Coalescence in Solid-Stabilized Emulsions,Eur. Phys. J. E., 11, 273 (2003).
29F. S. Ortega, P. Sepulveda, M. D. M. Innocentini, and V. C. Pandolfelli,Surfactants, a Necessity for Producing Porous Ceramics, Am. Ceram. Soc. Bull.,80  3742 (2001). &
September 2008 Cellular Ceramics by Direct Foaming 2829